Reclamation of Fibres from Rags : I—Identification of Non-carbonisable Fibres
Post on 30-Sep-2016
Sept. 1957 ATKINSON AND SPEAKMAN- RECLAMATION OF FIBRES FROM RAGS- I 41 7
Reclamation of Fibres from Rags I- Identification of Non-carbonisable Fibres
J. C. ATKINSON and J. B. SPEARMAN
Staining tests to distinguish between carbonisable, non-carbonisable, and protein fibres, and between the chief non-carbonisable fibres, have been developed. The fibres are treated with a mixture of fluorescent compounds, in presence of a stripping agent if dyed, and are then examined in ultraviolet radiation. In a few caaes, notably when the non-carbonisable fibres are heavily dyed black, stripping should precede staining.
In the past, when the fibres most likely to be mixed with wool were cotton and viscose rayon staple fibre, the recovery of wool for re-use presented little difficulty, because the cellulosic fibres are readily attacked by acids and can be removed, with little damage to the wool, by treatment with hot gaseous hydrogen chloride. Some difficulty was encountered with fabrics containing silk, and in so far as the latter was replaced by rayon, it might be claimed that the advent of man-made fibres was a t f i s t beneficial to the low-woollen industry. But then came the development of cellulose acetate, nylon, Terylene, and Orlon, all of which resist destruction by acids, and the growing use of blends of wool and staple fibres of these kinds is a cause of serious concern in the low-woollen industry. There is a t present no satisfactory commercial method of recovering wool from such blends for re-use, either by destroying the second component or, better, since the newer man-made fibres are of similar value to wool, by separating the components of the blend without destroying either.
It seems unlikely that any single process will be found capable of separating the component fibres of all blends, and a rapid method of identifying the non-carbonisable fibres present is clearly needed in order to facilitate classification for subsequent treatment. One possibility, which is the subject of this paper, is to treat the materials with a solution containing several fluorescent compounds, each having an aeni ty for some particular man-made fibre, and then to identify the latter by the colour of the fluorescence in ultra- violet radiation. Dyes were chosen as the fluorescent compounds to give additional ease of identification of undyed fibres, but it was hoped that dyed materials might be classified, after staining but without stripping, by examination in ultraviolet radiation.
Experimental UNDYED FIBRES
In relation to the processes of the low-woollen industry, the fibres present in rags may be regarded as falling into three groups, viz. cellulosic fibres, which are carbonisable, non-carbonisable man-made fibres, and protein fibres. At first, therefore, attention was focussed on the pre- paration of a mixture of dyes which would distinguish sharply between the three groups, the assumption being that any protein fibres present would normally be wool or a related animal fibre. Failure to discriminate between wool and
fibres such as Arciil and Fibrolane was regarded as unimportant, because the dyeing properties of these man-made fibres are similar to those of wool, and, in admixture with wool, the fibres promote milling shrinkage.
The selection of dyes for inclusion in the mixture was based on the inclusion of an acid dye for protein fibres, a basic dye for Orlon, and disperse dyes for cellulose acetate, nylon, and Terylene. Dyes of suitable colours were chosen after staining tests had been carried out with 1% solutions of some twenty fluorescent dyes in 40% alcohol. In addition, a fluorewent brightening agent was added to provide a sharp distinction between carbonisable and other fibres. Finally, in order to avoid compli- cations due to the presence of fatty matter in the materiaIs tested, a non-ionic detergent was added to the mixture, so that the fibres could be cleaned during the test itself, and the pH was adjusted to give effective discrimination between the three classes of fibre. A lengthy series of trials with
TABLE I Colours observed with Reagent A
Class Fibre Colour in Daylight Ultra-
Carbonisable Cotton Yellowish green
Viscose rayon Yellowish green
Cuprammonium Yellowish rayon green
Rayolanda Yellowish (Courtaulds) green
Non- Secondary Yellowish Green carbonisable cellulose green
acetate Nylon Pale Deep
Terylene (ICI) Very pale Bluish orange yellow
yellowish green green
green Orlon (DuP) Yellowish Green
Protein Fibrolane Deep red Deep red
Ardil (ICI) Deep red Deep red Wool Bluish red Bluish red
various dyes in different proportions and con- centrations led to the selection of the following midure-
418 ATKINSON AND BPEAKMAN- RECLAMATION O F FIBRES FROM RAGS- I J.S.D.C. 73
REAQENT A Duranol Brilliant Yellow 6G 300 16 ml. of 0.1% soh.
powder (C.I. Disperse Yellow 13) Acronol Yellow TC 180 (C.I. Basic 10 ml. of 0.1% soln.
Yellow 1) Sulphorhodamine B (C.I. Acid Red I 8 ml. of 0.1% soln.
52) Blancol BT (C.I. Fluorescent 20 ml. of 0.1% soh.
Lissapol N (ICI) 1 ml. Sulphuric acid (1.0 N.) 1 ml. Water 138 ml.
Brightening Agent 63)
When fibres are boiled in Reagent A for 2 min., and then washed thoroughly with water, the colom listed in Table I are obtained, examination under ultraviolet radiation being made with a mercury discharge unit giving 95% of its radiation at 3 6 5 0 ~ . If, then, a blend is found to contain fibres which are not coloured red, and which do not give a brilliant blue fluorescence in ultraviolet radiation, it may be concluded that non-carbonis- able man-made fibres are present.
The nature of the non-carbonisable fibres is not sharply defined by Reagent A, but they are readily identified by Reagent B, which is prepared by mixing 1% solutions in 40% alcohol of the following compounds in the specified proportions-
REAGENT B Parts (vol.)
Duranol Brilliant Yellow 6G 300 powder (C.I. 3
Lissamine Flavine FFS (C.I. Acid Yellow 7) 3
Blancol BT (C.I. Fluorescent Brightening Agent 3
Disperse Yellow 13)
Rhodnmine 3 (C.I. Basic Violet 10) 5
When fibres are treated with Reagent B at room temperature for 20 min., and then washed in water, the colours shown in Table I1 are obtained.
TABLE I1 Colours observed with Reagent B
Fibre Colour in Daylight Ultraviolet
Radiation Secondary cellulose Orange Deep yellow
Nylon Greenish yellow Green Terylene White Blueviolet Orlon Pink Red
In order to discover whether Reagent A could be used successfully with dyed fibres, tests were carried out with dyed samples of viscose rayon, cellulose acetate, nylon, and wool. Lightly dyed materials were readily classified as carbonisable, non-carbonisable, and protein, but the colour of the fluorescence was sometimes different from that obtained with undyed fibres, because the mercury discharge unit gave some visible light. Heavily dyed and dark-coloured materials, how- ever, gave no fluorescence, and it was recognised that stripping would be necessary before dyed materials could be identified. It was still hoped that a superficial strip would be sufficient to permit identification with fluorescent compounds,
whereas an almost perfect strip is essential when normal methods of staining are used; and if only mild stripping is required, it should be possible to carry out stripping and staining with a single reagent.
Of the stripping agents available, Formosul (Br) was selected as the most suitable. It was first shown that undyed fibres could be stained satis- factorily with the mixture of Duranol Brilliant Yellow 6G, Acronol Yellow TC, Sulphorhodamine B, and Blancol BT to which Formosul and acetic acid had been added. Among the non-carbonisable fibres, little difficulty was encountered with cellulose acetate and nylon, but Terylene and Orlon were more troublesome. With the latter fibres, improved results were obtained by including a swelling agent, Tumescal D (ICI), in the com- bined stripping and staining reagent. Unfortu- nately, an emulsion of Tumescal D must be prepared separately a t a temperature above 85"0., and the temperature of the reagent to which it is added must also be 8 5 " ~ . or above. It was found more convenient, therefore, to use rn-cresol as the swelling agent, emulsification being brought about with Dispersol A (ICI), which has the advantage of assisting the removal of disperse dyes from cellulose acetate and emulsifying any fatty matter present on the fibres.
The final composition of Reagent C, for use with dyed fibres, was as follows-
REAQENT C Duranol Brilliant Yellow 6G1 300
powder (C.I. Disperse Yellow 13) Acronol Yellow TC 180 (C.I. Basic
Yellow 1) Sulphorhodamine B (C.I. Acid Red
62) Blancol BT (C.I. Fluorescent
Brightening Agent 63) Dispersol A m-Cresol Acetic acid (30%) Water Formosul (C.I. Reducing Agent 2)
15ml. of 0.1% soln.
10 ml. of 0.1% soln.
18 ml. of 0.1% soln.
20 ml. of 0.1% soh.
40 ml. of 2.0% soln. 1 ml. 2 ml.
97 nil. 2 g.
The reagent is prepared by mixing the solutions of Duranol Brilliant Yellow 6G and Dispersol A and heating until the mixture clears, when the solutions of Acronol Yellow TC, Sulphorhodamine B, and Blancol BT are added. The water and the m-cresol are then heated in a separate vessel to give a clear solution, which is added to the warm solution of the dyes. After the mixture has cooled, acetic acid is added, and the volume adjusted to 200ml. The Formosul is added to the solution just before use, the dyed material under examina- tion being immersed in the cold solution, which is then raised to the boil.
Tests were made on fibres which had been dyed with a. wide range of dyes of various types-viz. disperse and basic dyes on cellulose acetate; acid, basic, and disperse dyes on nylon; disperse dyes on Terylene; basic and acid dyes (cuprous ion method) on Orlon; and acid, basic, azoic, and mordant dyes on wool. No special attention was paid to carbonisable fibres, because it is the detection of non-carbonisable fibres which is important. With
S~!pl. 1957 ATKINSON AND SPEAKMAN- RECLAMATION O F FIBRES FROM RAGS- II 419
pde dyeings on cellulose acetate, nylon, and Orlon the fibres could be identified after 2-15 min. boiling; but 25min. boiling was needed with Terylene, and ulth other fibres when they were heavily dyed. Similar results were obtained with the available range of commercial fabrics dyed with unknown types of dye, the non-carbonisable fibres giving a yellowish-green fluorescence.
Cases likely to cause special difficulty were also examined, e.g. heavy dyeings of mordant dyes on nylon and wool, and of azoic dyes on Terylene. When dyed with 8% Solochrome Black WDFA or 6BN (C.I. Mordant Black 11 or 3), for example, nylon gave no fluorescence after treatment with Reagent C, and only slight fluorescence when dyed with Solochrome Black F or PV 200 (C.I. Mordant Black 5 or 9). In such cases, stripping with a 2% solution of potassium dichromate in 1.0 N. sulphuric acid for 34min. , or with a 0.25% solution for 12-15 min., and then boiling for a few minutes in a 1% solution of Irgalon BT (Gy) to remove chromium, gave fibres which, after treatment with Reagent C, showed strong green fluorescence.
In the case of Terylene heavily dyed with azoic dyes, e.g. 6% Dispersol Diazo Black and 6% Brentosyn BB, it was found necessary to boil the material with a solution containing 0.5% sodium chlorite, 3% acetic acid (30y0), and 0.2% Tumescal D for 25 min. before sufficient stripping was obtained to allow the fibres to assume a green fluorescence on being treated with Reagent C.
Finally, although the detection of non-carbonis- able man-made fibres is the chief concern of this paper, mention should be made of the fact that no fluorescence could be obtained with heavily dyed
cotton, especially when Sulphur Blacks had been used, though good results were generally obtained with viscose rayon and Reagent C.
Conclusion The classification of undyed fibres as cnrhoniw-
able, non-carbonisable, and protein, and the identification of non-carbonisable fibres, can be carried out easily and quickly with Reagents A and B. Most dyed fibres can be classified and identified with equal certainty by means of Reagent C, which contains Formosul as the stripping agent. When, however, the fibres are heavily dyed, and especially when they are dyed black, more severe methods of stripping must be used before fluorescence can be developed with Reagent C. This is unfortunate, because it means that, when Reagent C fails to reveal the presence of non- carbonisable fibres, supplementary tests must be applied before their absence can be taken as certain. Although staining with fluorescent com- pounds has not, therefore, proved to be as infallible a test for non-carbonisable fibres as was at first hoped, Reagent C will, it is believed, find con- siderable use in the low-woollen industry.
* * * The authors are indebted to the Wool Textile
Research Council for financial assistance, and to Dr. C. B. Stevens for a number of helpful dis- cussions. TEXTILE CHEMISTRY LABORATORY
THE UNIVERSITY LEEDS 2
DEPARTMENT OF TEXTILE INDUSTRIES
(Received 5th February 1957)
Reclamation of Fibres from Rags 11-The Isolation of Wool from Mixtures of Wool and Terylene
J. C. ATKINSON and J. B. SPEAKMAN Wool may be recovered from mixtures of Terylene and wool by treatment with a 2% solution of
Whereas Terylene is completely destroyed under these hydrazine in butanol at 100"~ . for 60 min. conditions, the wool suffers only slight damage.
When the different fibres in rags are comparable in value, the ideal method of processing is clearly one in which all types of fibre are separated and recovered for re-use. The non-carbonisable fibres which are commonly mixed with wool have one property in common, viz. a low affinity for water, and any general method of separating wool from blends containing cellulose acetate, nylon, Terylene, and Orlon must be based on this property or on some closely related property, such as ease of electrification by friction I. Attempts to devise such a process have so far proved unsuccessful, and until one is available the less desirable method of destroying the non-carbonisable components of a blend in order to recover the wool for re-use must be adopted. The purpose of this investigation was to devise a method, of this kind for mixtures of wool and Terylene, a case which has a special interest because of the increasing use of Terylene
staple fibre in conjunction with wool, and because of the difficulty of dyeing fabrics made from reclaimed fibres in such a way as to mask the presence of Terylene.
Although a polyester, Terylene shows a sur- prisingly high resistance to attack by alkalis because of its high crystallinity; attack proceeds from the outside inwards, and a 4% solution of sodium hydroxide causes a loss in weight of only 20% in 80 min. at 100"~. Since wool is completely destroyed under the same conditions, alkalis seem hardly likely to merit serious consideration as a means of isolating wool from mixtures of wool and Terylene. There is, however, one case which deserves special consideration: esters are readily degraded by hydrazine, with liberation of the alcohol and formation of the hydrazide of the acid-
and Terylene should be attacked rapidly, in spitc R.CO0.R' + H,N*NH, -+ R.CO-NH*NH, + R'*OH